High Temperature VARTM of Phenylethynyl Terminated Imides
Depending on the part type and quantity, fabrication of composite structures using vacuum-assisted resin transfer molding (VARTM) can be more affordable than conventional autoclave techniques. Recent efforts have focused on adapting VARTM for the fabrication of high temperature composites. Due to their low melt viscosity and long melt stability, certain phenylethynyl terminated imides (PETI) can be processed into composites using high temperature VARTM (HT-VARTM). However, one of the disadvantages of the current HT-VARTM resin systems has been the high porosity of the resultant composites. For aerospace applications, the desired void fraction of less than 2% has not yet been achieved. In the current study, two PETI resins, LaRC PETI-330 and LaRC PETI-8 have been used to make test specimens using HT-VARTM. The resins were infused into ten layers of IM7-6K carbon fiber 5-harness satin fabric at 260 or 280 °C and cured at temperature up to 371 °C. Initial runs yielded composites with high void content, typically greater than 7% by weight. A thermogravimetric-mass spectroscopic study was conducted to determine the source of volatiles leading to high porosity. It was determined that under the thermal cycle used for laminate fabrication, the phenylethynyl endcap was undergoing degradation leading to volatile evolution. This finding was unexpected as high quality composite laminates have been fabricated under higher pressures using these resin systems. The amount of weight loss experienced during the thermal cycle was only about 1% by weight, but this led to a significant amount of volatiles in a closed system. By modifying the thermal cycle used in laminate fabrication, the void content was significantly reduced (typically ∼ 3% or less). The results of this work are presented herein.
High Temperature Transfer Molding Resins: Laminate Properties of PETI-298 and PETI-330
Two phenylethynyl terminated oligomers designated PETI-298 and PETI-330 were developed at the NASA Langley Research Center and have emerged as leading candidates for composite applications requiring high temperature performance (i.e. ≥ 288 °C for 1000 hours) combined with the ability to be readily processed into composites without the use of an autoclave or complex or lengthy cure or postcure cycles. These high performance/high temperature composites are potentially useful on advanced aerospace vehicles in structural applications and as aircraft engine components such as inlet frames and compressor vanes. The number designation (i.e. 298, 330) refers to the glass transition temperature in degrees Centigrade as determined on neat resin cured for 1 hour at 371 °C. The resins are processable by non-autoclave techniques such as resin transfer molding (RTM), vacuum assisted RTM (VARTM) and resin infusion (RI). Both resins exhibit low complex melt viscosities (0.1-10 poise) at 280 °C and are stable for ≥ 2 hours at this temperature. Typically, the resins are melted, de-gassed and infused or injected at 280 °C and subsequently cured at 371 °C for 1-2 hours. Virtually no volatiles are evolved during the cure process. The resin synthesis is straightforward and has been scaled-up to 25 kg batches. The chemistry of PETI-298 and PETI-330 and the RTM AS-4 and T-650 carbon fabric laminate properties, and those of BMI-5270 for comparison, are presented.
Effects of the mineral phase and valence of vanadium on vanadium extraction from stone coal
The influence of roasting on the leaching rate and valence of vanadium was evaluated during vanadium extraction from stone coal. Vanadium in stone coal is hard to be leached and the leaching rate is less than 10% when the raw ore is leached by 4 mol/L H2SO4 at 90°C for 2 h. After the sample is roasted at 900°C for 2 h, the leaching rate of vanadium reaches the maximum, and more than 70% of vanadium can be leached. The crystal of vanadium-bearing mica minerals decomposes and the content of V(V) increases with the rise of roasting temperature from 600 to 900°C, therefore the leaching rate of vanadium increases significantly with the decomposition of the mica minerals. Some new phases, anorthite for example, form when the roasting temperature reaches 1000°C. A part of vanadium may be enwrapped in the sintered materials and newly formed phases, which may impede the oxidation of low valent vanadium and make the leaching rate of vanadium drop dramatically. The leaching rate of vanadium is not only determined by the valence state of vanadium but also controlled by the decomposition of vanadium-bearing minerals and the existence state of vanadium to a large extent.